- Nano Express
- Open Access
Scanning tunneling spectroscopy of epitaxial graphene nanoisland on Ir(111)
© Phark et al.; licensee Springer. 2012
- Received: 9 January 2012
- Accepted: 17 April 2012
- Published: 15 May 2012
Scanning tunneling spectroscopy (STS) was used to measure local differential conductance (dI/dV) spectra on nanometer-size graphene islands on an Ir(111) surface. Energy resolved dI/dV maps clearly show a spatial modulation, which we ascribe to a modulated local density of states due to quantum confinement. STS near graphene edges indicates a position dependence of the dI/dV signals, which suggests a reduced density of states near the edges of graphene islands on Ir(111).
- Scanning Tunneling Microscopy
- Spatial Modulation
- Scanning Tunneling Microscopy Image
- Epitaxial Graphene
- Scanning Tunneling Spectroscopy
Graphene (G) has attracted significant attention because of its special and unique physical properties which make it a promising future material for nanoelectronics . In nanosize G structures, confinement geometry and increased edge-to-area ratio are expected to influence the electronic properties of G significantly. Previous studies showed how confinement of carriers in a G nanostructure affects the electrical conductivity  and the energy gap . Edge-localized electrons near the zigzag edge of a freestanding G nanoribbon were proposed by Nakada et al. . Recently, C. Tao et al.  reported electronic edge states dependent on the edge atomic orientations in G nanoribbons.
A theoretical study  predicted a small binding energy of ≈ 50 meV per C atom in G/Ir(111). G π-band related features were observed in angle-resolved photoemission spectroscopy studies of G/Ir(111) . However, a strong edge-substrate interaction in G nanoislands on Ir(111) has been proposed . This motivates a spatially resolved investigation of spectroscopic features of G/Ir(111) nanostructures to elucidate the spatial dependent electronic properties and the influence of the substrate on the electronic states near a G edge, and corresponding results are presented here.
We present scanning tunneling microscopy (STM) and scanning tunneling spectroscopy (STS) measurements on G nanoislands on Ir(111). The dI/dV spectra and maps show a spatial modulation, indicative of a modulated local density of states (DOS), which is ascribed to electronic quantum confinement . STS near the edge of a G island on Ir(111) shows a reduction of the differential conductance dI/dV. This reflects a change of the G electronic structure, which we ascribe to the different G-Ir interaction near the edge as compared to the central region of the G island.
Monolayer G islands were grown by exposing a clean and atomically flat Ir(111) surface to C2H4 at 300 K at a pressure of 2 × 10− 9 mbar, followed by subsequent heating of the substrate to 1,320 K. STM and STS measurements were performed at 8 K . Constant current (CC)-STM images showed that the island diameter ranges from 6 to 50 nm. We employed a lock-in technique with a modulation bias voltage at a frequency ν = 4 kHz and root-mean square amplitude of 20 mV to detect I(V) and dI/dV simultaneously.
We measured the dI/dV maps of the G island in Figure 1b as a function of V S . Figure 1d,e,f shows the dI/dV maps at V S denoted by the gray arrows in Figure 1g. As we lower V S from zero bias, the first modulation pattern (Figure 1d) is observed at V S ≈ − 0.44 V of peak ‘1’ of the dI/dV curve measured at position a. Here, the dI/dV signal shows a maximum at the center of the island and a monotonic decrease towards the edges. For larger negative V S , the maps at two other V S values (peaks ‘2’ and ‘3’) show different spatial distributions of the dI/dV signals as compared with that of the first one. These results can be understood as standing wave patterns which resulted from the interference of electron waves. The energy-dependent variation of the spatially modulated dI/dV signal suggests a variation of the electron wavelength as a function of electron energy in the G nanoisland. Thus, the position-dependent STS spectra and spatially modulated dI/dV signals provide a clear evidence for electron confinement in the G nanoisland. The energy eigenvalues of the confined electron states are determined by the geometry of the confinement potential (the size and shape of the island). This is also true for the graphene nanoislands . We observed a different onset energy of the lowest quantum-confined state (the first peak) in other graphene islands with different shape and size. We performed an extensive quantitative analysis of modulation patterns on G islands and extracted the electron dispersion relation .
Lacovig et al.  discussed, based on ab initio calculations, that the interaction between a G edge and Ir is strong enough to induce a considerable reduction (approximately 50%) of the C-substrate distance near the edges as compared with that of the central region of a G island on Ir(111). This structural relaxation should also impact the electronic DOS near an edge as compared to the central region of an island. The reduction of the dI/dV signal in Figure 2, which can be attributed to the reduction of the G DOS at the edges, possibly reflects this. We speculate that an unsaturated σ orbital at the edge tends to bond to the Ir atoms with a covalent character, which would reduce the edge energy and deplete the DOS near E F . This could explain the decrease of dI/dV signals in Figure 2. In addition, the electronic relaxation due to a C-Ir interaction at the edge could be the reason why our STS measurements do not show peculiar electronic states in the edge region, in contrast to the prediction of theory for the edge of freestanding G .
We investigated electronic properties of G nanoislands on Ir(111) by STM and STS. The dI/dV spectra and maps show a pronounced spatial modulation, indicative of a modulated local DOS. We ascribe this to a quantum confinement of electrons in G nanoislands. We also performed STS near the edge of a G island on Ir(111). Spatially resolved tunnel spectroscopy indicates a considerably reduced density of states. This reflects a change of the G electronic structure, which we ascribe to the different G-Ir interaction near the edge as compared to the central region of the G island.
This work was partially supported by Deutsche Forschungsgemeinschaft grant SFB 762. We thank N Kurowsky for the expert technical support.
- Castro Neto AH, Guinea F, Peres NMR, Novoselov KS, Geim AK: The electronic properties of graphene. Rev Mod Phys 2009, 81: 109–162. 10.1103/RevModPhys.81.109View ArticleGoogle Scholar
- Berger C, Song Z, Li X, Wu X, Brown N, Naud C, Mayou D, Li T, Hass J, Marchenkov AN, Conrad EH, First PN, de Heer WA: Electronic confinement and coherence in patterned epitaxial graphene. Science 2006, 312: 1191–1196. 10.1126/science.1125925View ArticleGoogle Scholar
- Ritter KA, Lyding JW: The influence of edge structure on the electronic properties of graphene quantum dots and nanoribbons. Nat Mater 2009, 8: 235–242. 10.1038/nmat2378View ArticleGoogle Scholar
- Nakada K, Fujita M, Dresselhaus G, Dresselhaus MS: Edge state in graphene ribbons: nanometer size effect and edge shape dependence. Phys Rev B 1996, 54: 17954–17961. 10.1103/PhysRevB.54.17954View ArticleGoogle Scholar
- Tao C, Jiao L, Yazyev OV, Chen YZ, Feng J, Zhang X, Capaz RB, Tour JM, Zettl A, Louie SG, Dai H, Crommie MF: Spatially resolving edge states of chiral graphene nanoribbons. Nat Phys 2011, 7: 616–620. 10.1038/nphys1991View ArticleGoogle Scholar
- Busse C, Lazić P, Djemour R, Coraux J, Gerber T, Atodiresei N, Caciuc V, Brako R, N’Diaye AT, Blügel S, Zegenhagen J, Michely T: Graphene on Ir(111): physisorption with chemical modulation. Phys Rev Lett 2011, 107: 036101.View ArticleGoogle Scholar
- Kralj M, Pletikosić I, Petrović M, Pervan P, Milun M, N’Diaye AT, Busse C, Michely T, Fujii J, Vobornik I: Graphene on Ir(111) characterized by angle-resolved photoemission. Phys Rev B 2011, 84: 075427.View ArticleGoogle Scholar
- Lacovig P, Pozzo M, Alfé D, Vilmercati P, Baraldi A, Lizzit S: Growth of dome-shaped carbon nanoislands on Ir(111): the intermediate between carbidic clusters and quasi-free-standing graphene. Phys Rev Lett 2009, 103: 166101.View ArticleGoogle Scholar
- Phark S, Borme J, León Vanegas A, Corbetta M, Sander D, Kirschner J: Direct observation of electron confinement in epitaxial graphene nanoislands. ACS Nano 2011, 5: 8162–8166. 10.1021/nn2028105View ArticleGoogle Scholar
- Li J, Schneider WD, Crampin S, Berndt R: Tunneling spectroscopy of surface state scattering and confinement. Surf Sci 1999, 422: 95–106. 10.1016/S0039-6028(98)00890-5View ArticleGoogle Scholar
- Kliewer J, Berndt R, Crampin S: Scanning tunneling spectroscopy of electron resonators. New J Phys 2001, 3: 22.View ArticleGoogle Scholar
- Hämalainen SK, Sun Z, Boneschanscher MP, Uppstu A, Ijäs M, Harju A, Vanmaekelbergh D, Liljeroth P: Quantum-confined electronic states in atomically well-defined graphene nanostructures. Phys Rev Lett 2011, 107: 236803.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.